PHYSICAL REVIEW B 75, 033316 2007
Zero g factors and nonzero orbital momenta in self-assembled quantum dots
Department of Physics, Fudan University, Shanghai 200433, China
and Institute for Microstructural Sciences, National Research Council, Ottawa, Ontario, Canada K1A 0R6
Institute of Experimental Physics, Warsaw University, Hoza 69, 00-681 Warszawa, Poland
Received 8 December 2006; published 26 January 2007
We point out using an empirical tight-binding approach that the ground state of holes in InAs/GaAs
self-assembled quantum dots carries nonzero orbital momentum. The spin and orbital motions of the hole state
are found to have opposite contributions to the hole g factor, leading to zero g factors of holes and then
excitons in dots of high aspect ratio. The nonzero envelope orbital momenta of the holes are also shown to
account for anisotropic circular polarization of exciton emission and nonlinear Zeeman splittings in high
magnetic fields. Our theory well explains recent experiments and indicates the possibility of engineering
magnetic splitting by tuning the electric confinement in nanostructures.
PACS numbers: 71.18.y, 78.67.Hc, 73.21.La
As one of the most important magnetic properties of a
system, the g factor measures the Zeeman splitting of an
electron state in a magnetic field and is determined by both
the spin and orbital motion of the electron. In semiconductors
like InAs and GaAs, the orbital motion of localized p
orbitals is strongly coupled to the spin, and the resulting
valence-band states can be classified by the corresponding
total angular momentum. Heavy and light holes, identified
by their different angular momenta, have distinctive g factors,
i.e., g hh =−6 and g s lh =−2 where is an empirical
parameter in the k· p theory. 1
In addition to the orbital motion of localized atomic orbitals,
electrons in nanostructures like self-assembled quantum
dots 2 can also acquire orbital magnetic moment due to
the motion around the circumference of the structures. However,
it is often taken for granted that the ground state of a
single exciton in these artificial atoms does not carry any
nonzero orbital momenta largely because the lowest level of
a natural atom is known to always have zero orbital momentum.
Such ignorance of the orbital motion can greatly impede
the understanding of electron and hole g factors in
quantum dots. 3
While it is true that the ground state of electrons in quantum
dots does not carry any angular momentum, we find that
the ground state of holes does carry nonzero envelope angular
momenta. In the present work, we will show that the
nonzero envelope orbital momenta NEOM of holes is essential
to understand the behavior of g factors of holes and
excitons and can explain the zero exciton g factor and nonlinear
Zeeman splittings observed in a recent experiment.
Moreover, we predict that the NEOM would lead to anisotropic
circular polarization of the exciton emission.
For the purpose of this study, we choose an sp 3 tightbinding
method 4 which has been successfully applied in ferromagnetic
quantum wells. 5 The one-electron tight-binding
Hamiltonian describes an electron hopping from atomic spin
orbital , at position R to spin orbital , at position
H tb =
where c R,,
HR,,;R,,c R,, c R ,,,
c R ,, are creation annihilation operators.
The basis of the spin orbitals is chosen as
s ↓ ,x ↓ ,y ↓ ,z ↓ ,s ↑ ,x ↑ ,y ↑ ,z ↑ . The hopping matrix
elements and site energies for s and p orbitals are extended
to include second-nearest-neighbor interactions 6 to fit the effective
masses of electrons and holes at the point and
conduction- and valence-band edges at both the and X
points exactly. Spin-orbit interaction is also incorporated.
In a magnetic field, Peierls phase factors are introduced to
transform the off-diagonal matrix elements as
HR,R → exp− i e R
Ardr HR,R, 2
where Ar is the vector potential. The Zeeman effect is
included by adding the spin terms to the diagonal matrix
HR ↑↓ ,R ↑↓ → HR ↑↓ ,R ↑↓ ± 1 2 g BB z ,
where g is the g factor of a bare electron. It is noted that no
additional empirical parameters like are used for the Zeeman
The calculations of electron and hole g factors are performed
for a typical lens-shaped InAs/GaAs quantum dot
which is 20 nm long in diameter, on a 2 monolayer wetting
layer and has a varying height. The total number of atoms
included in the calculation is about 500 000. A Lanczos algorithm
is used to compute the eigenvalues and eigenvectors
of large sparse matrices generated by the tight-binding
Hamiltonian. The calculation is first performed for the strain
distribution by an atomistic valence-force-field method, followed
by an analysis of the electronic structure by the tightbinding
©2007 The American Physical Society
PHYSICAL REVIEW B 75, 033316 2007
FIG. 1. Color online The Landé g factors of holes and electrons,
calculated as a function of the height of the lens-shaped selfassembled
InAs/GaAs quantum dots as shown in the inset. The
heights of the dots are in units of the lattice constant of GaAs.
Figure 1 plots the calculated hole and electron g factors,
g h and g e , as a function of the height of the dots. The result
exhibits a weak dependence of the electron g factor on the
height of the dots H. However, the hole g factor is found to
increase rapidly as the height H becomes larger. The combined
exciton g factor, g ex =g h +g e , is seen to change from
−1.47 when H3.4 nm to 0.09 when H6.2 nm. Hence,
the exciton g factor vanishes at a point between 10a and 11a.
In a recent magnetospectroscopy experiment of on single
InAs/GaAs quantum dots, 7 the exciton g factors of two
single dots were measured; one was about 3 nm high and
had g ex =−1.5 and the other was about 5 nm high and had an
almost zero exciton g factor, which nearly quantitatively
agrees with our theoretical calculation.
In the following, we will explain why the g factor of holes
and then excitons would vanish as the height of the dots
increases. Let us start with an analysis of valence-band states
in self-assembled quantum dots. Because of the influence of
the band mixing and strain field, the valence-band states in
quantum dots are much more complex than those in the conduction
bands. In general, a hole state in quantum dots is
composed of components from the heavy hh, light lh, and
split-off sh hole bands, and the conduction bands s. Itcan
be written as = n n↑ n ↑ + n↓ n ↓ , where n
=hh,lh,sh,s. 8–10 If only the contribution from the Bloch
functions is taken into account, the hole g factor can then be
expressed as g s h = n g n c n↑ −c n↓ , where g n is the g factor for
band n and c n = n n 2 . 11 Considering that the ground
state of the holes is dominated by its heavy and light hole
components, we have g s h g s hh c hh↑ +g s lh c lh↑ . It gives us a
simple theory to explain why the hole g factor becomes
smaller when the proportion of the heavy hole component
decreases, 12 which has been quite successful in quantum
wells where the lateral motion of carriers is not confined.
However, in quantum dots with strong lateral confinement,
understanding of the hole g factor would nevertheless require
knowledge of the spatial distribution of the envelope functions
of both heavy and light hole components.
Figure 2 plots the probability density of the light lh↑ 2
and heavy hh↑ 2 hole components in the ground state of
the holes in a dot of H=6a. The expectation value of the
FIG. 2. Color online Plots of light and heavy hole envelope
functions in the ground state of holes in a flat lens-shaped
InAs/GaAs quantum dot. The expectation values of the orbital momentum
operator L z are labeled.
orbital momentum operator in the envelope functions of the
light and heavy hole components can be calculated by Lˆ z
= h x/y−y/x h . Similar to the ground state of
the electrons, we find that the orbital momentum of the
dominant heavy hole component is very small L z 0.01.
However, the light hole components are found to carry nonzero
angular momenta, i.e., L z =0.99 for lh↑ and L z
=1.79 for lh↓ .
The reason why the heavy hole component of zero angular
momentum mixes with the light hole parts of nonzero
angular momenta lies in the fact that the total angular momentum,
i.e., the envelope part plus the Bloch part L z + j z ,
is a good quantum number in a system with cylindrical
symmetry. 8,9,13,14 Even if the symmetry is broken by the
shear strain, we find that the conservation of the total angular
momentum is still a good approximation.
Including the contribution from the envelope functions,
we have the overall hole g factor
g h = g h s + g h o ,
where g h o denotes the contribution from NEOM,
g o h =2 n↑ Lˆ zn↑
+ n↓ Lˆ zn↓
In the dot of flat shape as shown in Fig. 2, the light hole
components have a very small projection in the ground state
of holes, i.e., c lh↑ =1.86% and c lh↓ =0.41%; hence NEOM
give only a small contribution to the hole g factor. As the
light hole components take a larger proportion, the contribution
from the envelope part becomes more important to the
hole g factor.
Figure 3 plots the envelope orbital momenta of the heavy
and light hole components, i.e., hh↑ Lˆ zhh↑
/c hh↑ and
hh↑ Lˆ zlh↑
/c lh↑ , and g o h , as a function of the height of
dots. As the aspect ratio of the dot increases, the light hole
component is found to have a larger projection c lh↑ +c lh↓ in
the ground state of holes due to its stronger mixture with the
PHYSICAL REVIEW B 75, 033316 2007
FIG. 3. Envelope orbital momenta of the heavy and light hole
components in the ground state of holes and the corresponding
equivalent g factor calculated as a function of the height of the
lens-shaped self-assembled InAs/GaAs quantum dot as shown in
the inset of Fig. 1.
heavy hole part. 12 For example, when the height of the dot
H changes from 6a3.4 nm to 11a6.2 nm where a is
the lattice constant of GaAs, c lh↑ +c lh↓ increases from 2.0%
to 7.1%; in the meantime, the proportion of the heavy hole
part c hh↑ +c hh↓ drops from 96.6% to 89.0%.
Corresponding to these changes, the equivalent g factor
due to NEOM, g h o , becomes larger. Moreover, the heavy hole
component starts to gain noticeable NEOM when H8a,
which gives a significant contribution to g h o . For example, the
contribution from the heavy hole part alone accounts for
41% of g h o when H=9a while it increases to 61% when H
=11a. When the dot is flat, we find that the contribution from
NEOM g h o is small and the hole g factor is dominated by
that from the Bloch parts g h s . In this case, we have
g h o ≪g h s while g h s 0 and g h o 0. With the increase of the
aspect ratio of the dot, g h o becomes larger because of not only
the larger proportion of the light hole component but also the
NEOM of the heavy hole parts.
As the aspect ratio of the dot increases, the contribution
from the Bloch parts g h s is seen to become smaller while
that from the envelope orbital momenta g h o becomes the
dominant part in the hole g factor. Because the two parts g h
and g h o have the opposite signs, they are found to nearly
cancel each other when H=10a, which results in an almost
zero hole g factor. When the aspect ratio increases further,
g h o becomes larger than g h s , which leads to the change of
the sign of the overall hole g factor. At H=11a, the hole g
factor is found to become positive and nearly cancel the electron
g factor, leading to an almost zero exciton g factor,
which well explains the zero exciton g factor observed in the
recent experiment. 7
While the result shown in Fig. 2 may also be obtained by
the eight-band k· p method, 15 we find that it is necessary to
apply the tight-binding approach for the calculation of the g
factors. The key to this issue is that the parameter used in
the k· p theory is not well established. Even in quantum
wells, a fitting procedure is often required to reproduce the
experimental data, 16 and xxx the uncertainty in its value can
be as large as 10%. In our k· p calculation, a mere 3% change
in from 7.68 to 7.48 can induce a change of more than
FIG. 4. Color online The proportion of the heavy hole component
in the spin-up and spin-down states of the holes and the circular
polarization of the exciton emission, calculated as a function of
magnetic field in a lens-shaped InAs/GaAs quantum dot.
20% in the resulting hole g factor from 0.30 to 0.24. Another
difficulty we encounter in the k· p calculation is that in
most cases it gives electron and hole g factors with opposite
signs, 12 which is in an obvious contradiction with the experiment
where the electron and hole g factors are shown to have
the same sign. 3
Besides the zero g factors of holes and excitons, the interplay
between the contributions from the Bloch and envelope
parts g h and g o h can lead to many other observable
effects such as anisotropic circular polarization of the exciton
emission in a high magnetic field. Let us take the example of
the dot with height H=10a. As can be seen in Fig. 1, the
overall hole g factor nearly vanishes due to the opposite
contribution from the heavy and light hole parts. It can be
estimated that the effective g factor including both the
Bloch parts and NEOM for the heavy hole part is g hh
−0.07 and for the light hole part g lh 0.08. As the magnetic
field increases, the heavy hole part of the spin-up state tends
to lower its energy because g hh 0. In the meantime, its light
hole part tends to do the opposite since g lh 0. The competition
means that the spin-up state gains more heavy hole part
while losing the light hole part as the field increases. A similar
process also goes on in the spin-down state, but, ending
with the opposite dependence.
The calculated c hh↑ and c hh↓ are plotted as a function of
the magnetic field in Fig. 4, and exhibit the predicted dependence.
As the intensity of the + − transition is mainly
determined by the proportion of the heavy hole components
in the spin-up spin-down hole state, the polarized heavy
hole components directly lead to the anisotropic circular polarization
of the exciton emission. The calculated degree of
circular polarization defined 17 by p=I +−I −/I ++I − is
plotted in Fig. 4, and is seen to increase with the magnetic
field. It is noted that due to the spin relaxation effect, this
phenomenon may not be well resolved when linearly polarized
excitation is applied. Instead, circularly polarized excitation
should be used for the observation of this effect.
Another observable phenomenon induced by NEOM is
nonlinear Zeeman splittings. As the spin-down state is noticed
to lose its heavy hole component faster than the spin-up
state gains the heavy hole component, the total projection of
the heavy hole components in the spin-up and spin-down
hole states decreases as the magnetic field increases, which
causes the g factor of holes to change as the magnetic field
increases and leads to weak yet observable nonlinear Zeeman
NEOM also exist in other kinds of systems like carbon
nanotubes. 18 Although the motion of carriers is not confined
in the lateral directions in quantum wells, a magnetic field
applied along the growth direction would induce lateral orbital
motion that mixes heavy and light hole states. Such a
band mixture sometimes leads to strong nonlinear Zeeman
splitting. 16 In spite of some similarities between the orbital
motion in quantum dots discussed here and that induced by
the applied magnetic field in quantum wells, the difference is
obvious: NEOM in self-assembled quantum dots are induced
by the structural confinement and hence represent an intrinsic
property that does not depend on an external field. While
it may be argued that the mechanism leading to NEOM has
been included in previous work, 12 we would like to remind
the reader that NEOM have not been explicitly studied, let
alone their effect on the g factor of holes in quantum dots.
On the contrary, it has recently been reported that the behavior
of the hole g factor in quantum dots can be understood in
PHYSICAL REVIEW B 75, 033316 2007
terms of orbital momentum quenching, 19 which is proved
incorrect by our calculation.
As a result of NEOM, the light hole component in the
ground state of holes has almost zero overlap with the
ground state of electrons in a flat quantum dot; therefore, it
has little contribution to the interband transition. As the aspect
ratio increases, L z = lh L z lh − e L z e starts to
deviate from 1, which partially lifts the forbidden transition.
In conclusion, we find that the hole g factor has two distinct
contributions in self-assembled quantum dots, one from
the Bloch functions and the other from the nonzero orbital
momenta carried in the envelope functions of the holes. We
show that these two contributions to the hole g factor have
opposite signs and account for the zero g factors of holes and
excitons in dots of high aspect ratio. We also point out that
the nonzero orbital momenta are responsible for anisotropic
circular polarization of the exciton emission and nonlinear
This work is supported by the NSFC Nos. 10644001 and
10634040. The authors thank P. Hawrylak and M. Korkusinski
1 M. H. Weiler, in Semiconductors and Semimetals, edited by R. K.
Willardson and A. C. Beer Academic, New York, 1981, Vol.
16, p. 119.
2 D. Bimberg, M. Grundmann, and N. N. Ledentsov, Quantum Dot
Heterostructures Wiley, New York, 1999.
3 M. Bayer, A. Kuther, A. Forchel, A. Gorbunov, V. B. Timofeev,
F. Schäfer, J. P. Reithmaier, T. L. Reinecke, and S. N. Walck,
Phys. Rev. Lett. 82, 1748 1999; M. Bayer, A. Kuther, F.
Schäfer, J. P. Reithmaier, and A. Forchel, Phys. Rev. B 60,
4 S. J. Sun and Y.-C. Chang, Phys. Rev. B 62, 13631 2000.
5 I. Vurgaftman and J. R. Meyer, Phys. Rev. B 64, 245207 2001.
6 W. Sheng and P. Hawrylak, Phys. Rev. B 73, 125331 2006.
7 A. Babinski, G. Ortner, S. Raymond, M. Potemski, M. Bayer, W.
Sheng, P. Hawrylak, Z. Wasilewski, S. Fafard, and A. Forchel,
Phys. Rev. B 74, 075310 2006.
8 O. Stier, Ph.D. thesis, Berlin Studies in Solid State Physics Vol. 7
W&T, Berlin, 2000.
9 M. Grundmann, Nano-Optoelectronic: Concepts, Physics and Devices
Springer, Berlin, 2002.
10 W. Sheng, S.-J. Cheng, and P. Hawrylak, Phys. Rev. B 71,
11 A. V. Nenashev, A. V. Dvurechenskii, and A. F. Zinovieva, Phys.
Rev. B 67, 205301 2003.
12 T. Nakaoka, T. Saito, J. Tatebayashi, and Y. Arakawa, Phys. Rev.
B 70, 235337 2004; T. Nakaoka, T. Saito, J. Tatebayashi, S.
Hirose, T. Usuki, N. Yokoyama, and Y. Arakawa, ibid. 71,
13 U. Woggon, Optical Properties of Semiconductor Quantum Dots,
Springer Tracts in Modern Physics Vol. 136 Springer, Berlin,
14 L. G. C. Rego, P. Hawrylak, J. A. Brum, and A. Wojs, Phys. Rev.
B 55, 15694 1997.
15 W. Sheng and J.-P. Leburton, Phys. Status Solidi B 237, 394
16 N. J. Traynor, R. T. Harley, and R. J. Warburton, Phys. Rev. B 51,
7361 1995; N. J. Traynor, R. J. Warburton, M. J. Snelling, and
R. T. Harley, ibid. 55, 15701 1997.
17 A. Kuther, M. Bayer, A. Forchel, A. Gorbunov, V. B. Timofeev,
F. Schäfer, and J. P. Reithmaier, Phys. Rev. B 58, R7508 1998.
18 E. D. Minot, Yuval Yaish, V. Sazonova, and P. L. McEuen, Nature
London 428, 536 2004.
19 C. E. Pryor and M. E. Flatté, Phys. Rev. Lett. 96, 026804 2006.